- Nano Express
- Open Access
Synthesis, Characterization, Luminescent and Nonlinear Optical Responses of Nanosized ZnO
© The Author(s). 2017
- Received: 30 December 2016
- Accepted: 20 February 2017
- Published: 3 March 2017
In this study, we report soft and solvothermal methods for synthesis of zinc oxide nanoparticles (ZnO NPs). Both methods involve a precursor and are carried out at the middle low-temperature regime. The effect of different solvents on the ZnO NPs properties was studied. The nonlinear optical (NLO) response of the NPs was analyzed by the self-action of picosecond laser pulses at 1064 nm and by second harmonic generation (SHG) of a femtosecond laser pulses pump at 800 nm. The luminescence was studied within UV-visible ranges. It was shown that the NLO response efficiency significantly depends on the solvent. The obtained SHG efficiency of small (~2 nm) ZnO NPs is comparable to the one obtained for large (~150 nm) commercial ZnO NPs. The observed results are important for the application of the ZnO NPs in biolabeling.
- ZnO nanoparticles
- NLO response
- Remote optical diagnostics
- Second harmonic generation
Zinc oxide (ZnO) is one of the widely used materials. It is a low-cost semiconductor with a large bandgap (3.37 eV), high Wannier-Mott exciton binding energy (~60 meV), and promising luminescent properties [1–8]. The ZnO nanoparticles (NPs) and quantum dots (QDs) have found their application in the fields of sensing, LEDs, etc. They can be assembled with transparent conductive oxide waveguides for the realization all ZnO-based optoelectronic devices . However, there are a few reports on synthesizing of ZnO NPs or QDs with ultra-small size; these results are reviewed in . For this instance, the control synthesis of ZnO NPs is of interest because they possess electro-optical properties that differ from their bulk counterparts, being sensitive to both the NP’s size and shape.
Various methods [10–13], including synchrotron radiation-assisted spectroscopes [12, 13], have been reported for the characterization and theoretical modeling of wide bandgap oxide materials comprising defective and nanostructured ZnO [10, 11]. Chemical approaches for ZnO NPs preparation are the gas-phase techniques, sol-gel methods, evaporative decomposition of solutions, and wet chemical syntheses [1, 5]. In a mainstream of a large-scale synthesis, soft chemical methods can be chosen due to a low growth temperature and a good scale-up potential [2, 3].
To obtain small ZnO NPs, we have used a chemical method under a wet chemistry paradigm, which, by definition, involves stabilization of ZnO core with an organic amine [6, 14]. In this case, the used templating agent acted as a weak base promoting the formation of ZnO NPs . The NPs’ growth condition must be carefully chosen to minimize hydrolysis at the earliest stage, which determines the ZnO core size. The ZnO nucleation and NP growth should pass under the action of the equimolar amount of hydrolytic agent (H2O). This condition is satisfied in the case of zinc acetate dihydrate Zn(CH3COO)2 × 2H2O — the substrate capable of autohydrolysis. A cascade growth of ZnO NPs can be typically prevented by keeping the hydrolysis within the absolutized solvent medium. Taking into account the fact that higher substrate concentration causes smaller ZnO core size [15, 16], one can limit the growth rate basing on the cellular effect. Besides, a high concentration of acetate complex of zinc with an organic polyfunctional amine increases the viscosity of the solution and reduces the effective size of the cell. Therefore, sufficiently high concentrations of triethanolamine, which act as a stabilizing agent for the small ZnO NPs by adsorption on the surface, could limit the growth of the large oxide NPs.
The abovementioned arguments provide background for a proper choice of the seed mixtures for the NPs growth process. The properties of the resulted NPs were compared with the reference NPs obtained by solvothermal synthesis and the large commercial NPs (90–200 nm).
In the recent studies on harmonic nanoparticles , the ZnO NPs have shown a high potential for the application. Such NPs with an efficient nonlinear χ (2) response can be imaged via the second harmonic generation (SHG) effect as the contrast mechanism. The application in biolabeling requires the NPs size reduction (at least less than 100 nm) while maintaining the same level of the SHG efficiency.
In the present work, we provide the nonlinear optical (NLO) properties and SHG efficiency study of small ZnO NPs. Their density of defects and sizes were characterized with a range of spectroscopic techniques.
Reagents and Materials
Triethanolamine (TEA) was purchased from Merck. Sigma-Aldrich solvents isopropanol (i-PrOH), ethanol (EtOH), acetonitrile (MeCN), and propylene glycol (PPG) were dried with molecular sieves and distilled. Aldrich zinc acetate dihydrate (Zn(CH3COO)2 × 2H2O, ≥99%) was used as received. Commercial ZnO NPs (Nanostructured & Amorphous Materials Inc., Houston, USA) were purchased for comparison with the synthesized particles. They were specified to contain ZnO NPs of 90–200 nm in size.
The reference ZnO NPs were obtained using the thermal hydrolysis of Zn(CH3COO)2 × 2H2O in 1-hexadecanol (HD, ReagentPlus®, 99%, Sigma-Aldrich) smelt according to the protocol from . The thermal decomposition of ZnO precursors gives ZnO NPs with an average size of 50 nm.
The ZnO NPs were produced as follows: 5.56 g of TEA was dissolved in 100 ml of abs. solvent, viz. i-PrOH, EtOH, MeCN, and PPG. The resulting solution was added to 13.65 g of Zn(CH3COO)2 × 2H2O in Pyrex® glass autoclave. With constant stirring, the solution was heated to 60 °C for 2 h. At this time, there was a gradual coloring of the prepared solution to light or pale yellow during synthesis; see Additional file 1: Figure S1. A significant precipitation was observed upon cooling of the resulting solutions, excluding PPG. The dropped precipitates are colored pale yellow too. It was found that the hydrolysis at 60 °C gives the best coloration to the ZnO NPs solution. The growth of ZnO is accompanied by the luminescence inherent in NPs , under UV light at 365 nm (Additional file 1: Figure S2). Since the solution shows no Tyndall cone, it contains no ZnO colloidal suspensions.
The characterization of optical and nanostructural properties of prepared ZnO NPs was performed as follows. Ultraviolet-diffuse reflection (UV-DR) spectra of solid precipitates containing ZnO NPs and ultraviolet-visible (UV-Vis) adsorption spectra of ZnO NPs solutions were recorded with a scanning rate of 1 nm by UV-Vis spectrophotometer (Shimadzu UV-2700). Fourier transform infrared (FTIR) spectra were collected on a Thermo Nicolet Nexus 470 FTIR. Photoluminescence (PL) spectra of the ZnO NPs dispersed in solvents were measured at 25 °C using a spectrofluorimeter (PerkinElmer LS 55, Xe flash lamp). The excitation and emission spectra were recorded in the range 200–800 nm under optimal conditions at maximum wavelengths for each studied system. The spectral data were acquired using 0.5-nm step and 3-nm bandwidths for both emission and excitation monochromators. X-ray diffraction (XRD) patterns were registered with CuKα radiation on a Phillips PW 1800 diffractometer.
The NLO response of solid precipitates, obtained from i-PrOH, EtOH, CH3CN, and HD, were studied within the self-action of picosecond laser pulses (42 ps FWHM, repetition rate 15 Hz) at 1064 nm [20, 21]. The precipitates were placed into the bed with ∅ ~ 8 mm in the Teflon® film positioned between two glass microscope slides (Marienfeld, 76 × 26 × 1 mm3). The film thickness d = 340 μm was chosen to provide an optical homogeneity of the solid sample layer sufficient for the registration transmittance level. This approach is described in detail for the carbon material bulk particle NLO diagnostics .
The obtained total and on-axis transmittance dependencies on the peak intensity I are presented as the smoothed curves produced by local B-splines of the measured data. Each curve corresponds to ~5000 registered laser shots. The relative errors of the curves do not exceed 0.2% for the total and 1% for the on-axis transmittance dependencies correspondingly.
The sample was positioned at the distance of 14.5 cm from the focusing lens L with a focal distance of 11 cm. The scattered second harmonic (SH) signal readout was realized at 90° from the laser beam axis by Atik 16IC CCD camera. In order to cut the fundamental radiation and extract the SH signal, band-pass (BP, 405 nm, 10-nm FWHM) filter was positioned on the CCD camera. The energy of the incident pump pulses was measured by the photodiode PD.
Taking into account that the displacement energy for ZnO is higher than 55 eV , we do not expect the formation of new vacancies and interstitials under the applied regimes of laser excitation in the experiments.
The ZnO NPs prepared were analyzed by excitation-emission spectrofluorimetry technique. PL spectra of ZnO NPs in different solvents show a broad emission ranging from 400 to 600 nm with the emphasis in the violet-blue range, Fig. 2b. The PL spectra were deconvoluted into Gaussian peaks at about 2.3, 2.8, and 3.0 eV (539, 443, and 413 nm, respectively). Several bands of the PL signal cannot be attributed to the presence of different NPs since the adsorption of acetate and TEA should prevent small NPs from aggregation. The PL intensity decreases, in the range of used solutions, from EtOH to PPG. This result correlates with the NPs concentration and UV-Vis absorption (cf. Fig. 2a, b). PL properties of ZnO, in general, are very sensitive to defects. The most probable explanation of observed PL spectra is the presence of numerous energy levels. Typically, the levels originated from various defects, including vacancies and interstitials.
According to Ref. , the green emission at ~2.3–2.4 eV (539–516 nm) is addressed to the transition from the conduction band (CB) to the deep-level states assigned to the oxygen vacancies (OV) of the NP interface. The violet and blue emission peaks were addressed to other defects [27–29]. The peaks at ~413 and 443 nm could be attributed to transitions between the highest inter-node and the lowest valence band (VB) . Obviously, the intensive violet emission is due to defective zinc interstitial (Zn i ) levels. The observed blue emission could be addressed to the different defects even in zinc vacancies as reported in .
The high intensity of the PL emission (see the left insert in Fig. 2b) indicates a high density of extended defects in the ZnO structure. This fact once again accentuates a non-equilibrium character of the NPs formation process.
For the isolated ZnO NPs, two efficient absorption bands were observed at about 407 and 503 cm−1. The band at 407 cm−1 was assigned to Zn–O stretching vibration, while the band at 503 cm−1 can correspond to the oxygen deficiency in ZnO NPs . The H–O–H bending vibration mode is registered near 1620 cm−1. Asymmetric stretching vibrations of OH− groups are identified in the range of 3210–3670 cm−1. These observations provided the presence of hydration in the structure. One could suppose the NPs capping agents such as Ac− and TEA from the spectra comparison (Fig. 3a).
The UV-Vis spectra of solutions containing ZnO NPs and UV-DRS spectra of the co-precipitated mixture of the reagents and hydrolysis products (obtained from the same solutions) are similar (Additional file 1: Figure S3). A halo registered in the UV-DRS spectra is positioned in the same spectral range as bands in the UV-Vis spectra of ZnO NPs containing solutions that can be attributed to the ZnO NPs contribution.
where λ corresponds to the peak position and indicates larger ZnO NPs in the range of D from 2.0 to 2.8 nm. This means coagulation of ZnO NPs with the smaller size (D ~1.5–2.0 nm) after the temperature reduction to 16 °C. A small area of the absorption peak and plenty of precipitated solid indicate that the remaining concentration of the ZnO NPs is very low. The NPs growth process does not reach the stoichiometric composition of NPs cores that was confirmed by the blue emission at about 443–450-nm manifestation in the PL spectra (Fig. 2b). At the background of the stabilization with the same amine, the size of ZnO NPs is weakly dependent on the used solvents.
In contrast to the Brus equation  that can be applied for larger NPs of above 6 nm in diameter, the range of validity of Eqn. (2) covers the NPs sizes from D ~2.5 to 6 nm . However, in the present case, the value of E g was found within a range of 4.10 to 4.72 eV that corresponds to the NPs sizes varying from D ~1.8 to 1.2 nm, which is far below the recommended interval.
Summing up the observations collected during the preparation of the solid precipitates, we will briefly discuss the findings below. Undoubtedly, the ZnO NPs have the potential to be immobilized by occlusion — the incorporation of nanoparticles inside the growing solid. Typically, the precipitate, at the initial formation stage, captures the small ZnO NPs, of ca. 2–3 nm, contained in the solutions. The fast rate of the process prevents further NPs growth. It resulted in the formation of the solids containing defective ZnO NPs, which are similar to the ones reported in [34, 35]. In contrast to the small ZnO NPs, the solids with HD contains 50 nm ZnO covered with HD and the rest of the hydrolysis products.
In comparison to good-quality XRD patterns reported in [32, 36], the XRD patterns obtained in this work are mainly of a lower quality. We assume this is due to the semi-amorphous origin of the solids and a low content of ZnO NPs covered with a mixture of reagents and products.
PL and NLO parameters
Parameters of VO band
Peak position, eV
T 0, %
Re(χ (3)), ×10−9 esu
Im(χ (3)), ×10−11 esu
Figure 4a presents the photoinduced variations of the total transmittance of the solid precipitates, obtained from i-PrOH, EtOH, MeCN, and HD. It was shown the total transmittance variation in the studied peak intensity range to be slow. At the initial I ≤ 2 MW/cm2 range, the total transmittance was approx. constant (T 0) that corresponded to the linear regime of the optical transmittance. The T 0 magnitude significantly depends on the solvent; see Table 1. In the range of used solvents, the magnitude reduces in the following order HD > EtOH > i-PrOH > MeCN. To derive the photoinduced effect manifestation from the linear response of a background, we normalized the obtained dependencies (Fig. 4a) on a linear transmittance T 0. The results are shown in Fig. 4b as smoothed curves with the relative error of about ±0.2% .
Analysis of the presented data reveals non-monotonic photoinduced total transmittance variations in precipitates from EtOH, i-PrOH, and MeCN, while for the case of HD, monotonic photoinduced darkening was observed. For the peak intensity range >100 MW/cm2, the efficient photodarkening for all studied samples can be attributed to the two-photon resonant excitation of the VO. For this range, from the obtained dependencies, the imaginary part of the cubic NLO susceptibility Im(χ (3)) was estimated within the approach described in . The results are presented in Table 1. One can see the Im(χ (3)) magnitudes decrease in the following order EtOH > i-PrOH > MeCN that correlates with the VO band area, being proportional to the NPs concentration.
The on-axis transmittance dependencies reveal the different sign of the refractive NLO response for the ZnO NPs precipitates, obtained from different solvents. The photoinduced self-focusing effect was observed for MeCN and EtOH while the self-defocusing one for HD and i-PrOH. From the obtained dependencies, the real part of the cubic NLO susceptibility Re(χ (3)) was estimated . The observed Re(χ (3)) positive magnitudes for the ZnO NPs precipitates, obtained from MeCN and EtOH, can be explained by the two-photon resonant excitation of the oxygen vacancies. The two quanta energy 2.33 eV does not exceed the VO band spectral position (see Table 1) that determines the positive refractive NLO response of the trapped carriers . In this case, a more efficient refractive response of ZnO NPs in MeCN is dealing with better overlapping of the VO band position with the two-photon laser quanta energy.
The manifestation of the self-defocusing effect (Re(χ (3)) < 0) for the ZnO NP precipitate obtained from i-PrOH solutions requires more detailed study.
In order to compare the results, we analyzed the SHG efficiency in certain excitation ranges. The effective order p of the NLO response I 2ω ~ (I ω) p was estimated from the slope of the linear approximation of the presented dependencies. At peak intensity range 10–13 GW/cm2, the maximal p = 1.9 was obtained for the i-PrOH solution containing ZnO NPs. The synthesized and large ZnO NPs demonstrated lower p = 1.7 in the EtOH. Higher SHG efficiency in the small ZnO NPs instead of the large ones indicates the manifestation of the surface mechanisms on the background of the bulk response.
For I ω > 15 GW/cm2, we have observed higher SH magnitude from the larger NPs with p = 2.3. It can be explained by the cubic NLO response contribution into the SHG efficiency enhancement. The similar effect was observed in the KDP single crystals with incorporated TiO2 NPs .
The obtained result indicates the high brightness of the SHG signal of the synthetized novel small (~2 nm) ZnO NPs, making them promising for biolabeling application .
A set of the ZnO NPs with efficient luminescent and quadratic NLO responses was successfully prepared by the hydrolytic route. The ZnO NPs demonstrated the emission in the solution and in the solid state. The solutions and solid precipitates containing ZnO NPs were characterized with UV-Vis/UV-DRS and FTIR spectroscopy. Small ZnO NPs were stabilized at the early stages of hydrolysis by protecting NPs cores with adsorbates and limiting the particles’ growth. The analysis of UV-Vis absorption in the range of 330–350 nm revealed the obtained ZnO NPs sizes within 2.0–2.8 nm.
The PL emission and UV-Vis absorption manifestation with increases symbate with the concentration of ZnO NPs. It grows in the following order of the solvents EtOH > i-PrOH > MeCN > PPG. The violet, blue, and green PL band emissions from the solutions were addressed to the NPs with high-defect concentration.
The NLO characterization of the ZnO NPs containing precipitates was provided by the self-action effect monitoring within the picosecond laser pulses at 1064 nm. It was shown that the ZnO NPs containing precipitates obtained from different solvents produce a different efficiency of the absorptive and refractive NLO responses. The correlation between the Im(χ (3)) magnitudes and the area of the PL band at about 2.34–2.41 eV that related to the oxygen vacancies in ZnO was revealed. These results indicate high potential of the applied technique for the ZnO NPs diagnostics.
The second harmonic generation in the ZnO NPs was studied within the femtosecond laser excitation at 800 nm. It was shown that the SHG efficiency of the synthetized ZnO NPs (~2 nm) and the large commercial ZnO NPs (~150 nm) are comparable. The effect is important for the application of small ZnO NPs in biolabeling.
This work was partially supported by joint NASU-NASB project No. 04-02-15 and NASU project B/166. The work was partially performed at CCU IP NASU facilities.
VYaG supervised the project as the scientific group leader and principal investigator. VVL and OYuB conceived the idea of synthesis. ANZ and VOK did the synthesis. AVU and VVM performed the optical measurements and data analysis. VVL, VOK, and OYuB conducted the spectroscopic and analytic measurements. RPL carried out the PL measurements. All the authors analyzed and discussed the results. VYaG, AVU, and VVL wrote the manuscript. All authors read and approved the final manuscript.
The authors declare that they have no competing interests.
Open AccessThis article is distributed under the terms of the Creative Commons Attribution 4.0 International License (http://creativecommons.org/licenses/by/4.0/), which permits unrestricted use, distribution, and reproduction in any medium, provided you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made.
- Chetia TR, Ansari MS, Qureshi M (2016) Rational design of hierarchical ZnO superstructures for efficient charge transfer: mechanistic and photovoltaic studies of hollow, mesoporous, cage-like nanostructures with compacted 1D building blocks. Phys Chem Chem Phys 18:5344–5357. doi:10.1039/c5cp07687k View ArticleGoogle Scholar
- Mei T, Hu Y (2011) Synthesis, self-assembly and optoelectronic properties of monodisperse ZnO quantum dots, optoelectronic devices and properties, Ed. Sergiyenko O, InTech China, Shanghai, pp. 215–240. doi:10.5772/14389
- Sun X, Li Q, Jiang J, Mao Y (2014) Morphology-tunable synthesis of ZnO nanoforest and its photoelectrochemical performance. Nanoscale 6:8769–8780. doi:10.1039/C4NR01146E View ArticleGoogle Scholar
- Li X, Zhou X, Liu Y, Sun P, Shimanoe K, Yamazoe N, Lu G (2014) Microwave hydrothermal synthesis and gas sensing application of porous ZnO core–shell microstructures. RSC Adv 4:32538–32543. doi:10.1039/C4RA03789H View ArticleGoogle Scholar
- Maria MJ, Balanand S, Anas S, Mohamed AP, Ananthakumar S (2016) Zn-dust derived ultrafine grained ZnO non-linear ceramic resistors via in-situ thermal oxidation of cermet reactant mixture. Mater Design 92:387–396. doi:10.1016/j.matdes.2015.12.053 View ArticleGoogle Scholar
- Shi W, Song S, Zhang H (2013) Hydrothermal synthetic strategies of inorganic semiconducting nanostructures. Chem Soc Rev 42:5714–5743. doi:10.1039/C3CS60012B View ArticleGoogle Scholar
- Tonto P, Mekasuwandumrong O, Phatanasri S, Pavarajarn V, Piyasan P (2008) Preparation of ZnO nanorod by solvothermal reaction of zinc acetate in various alcohols. Ceram Int 34:57–62. doi:10.1016/j.ceramint.2006.08.003 View ArticleGoogle Scholar
- Jincheng Fan J, Li T, Heng H (2016) Hydrothermal growth of ZnO nanoflowers and their photocatalyst application. Bull Mater Sci 39:19–26. doi:10.1007/s12034-015-1145-z View ArticleGoogle Scholar
- Liu Y, Li Y, Zeng H (2013) ZnO-based transparent conductive thin films: doping, performance, and processing. J Nanomater 2013:196521. doi:10.1155/2013/196521 Google Scholar
- Liu Y, Kang ZH, Chen ZH, Shafiq I, Zapien JA, Bello I, Zhang WJ, Lee ST (2009) Synthesis, characterization, and photocatalytic application of different ZnO nanostructures in array configurations. Cryst Growth Des 9:3222–3227. doi:10.1021/cg801294x View ArticleGoogle Scholar
- Kaurova IA, Kuz’micheva GM, Rybakov VB, Cousson A, Gayvoronsky VY (2014) Structural peculiarities and point defects of bulk-ZnO single crystals. J Alloy Compd 616:71–75. doi:10.1016/j.jallcom.2014.07.027
- Balasubramanian C, Bellucci S, Cinque G, Marcelli A, Guidi MC, Piccinini M, Popov A, Soldatov A, Onorato P (2006) Characterization of aluminium nitride nanostructures by XANES and FTIR spectroscopies with synchrotron radiation. J Phys: Cond Matter 18:S2095. doi:10.1088/0953-8984/18/33/S25
- Popov AI, Shirmane L, Pankratov V, Lushchik A, Kotlov A, Serga VE, Kulikova LD, Chikvaidze G, Zimmermann J (2013) Comparative study of the luminescence properties of macro- and nanocrystalline MgO using synchrotron radiation. Nucl Instr Meth Phys Res B 310:23–26. doi:10.1016/j.nimb.2013.05.017
- Hu Z, Oskam G, Searson PC (2003) Influence of solvent on the growth of ZnO nanoparticles. J Colloid Interface Sci 263:454–460. doi:10.1016/S0021-9797(03)00205-4
- Feng ZC (2012) Handbook of zinc oxide and related materials: volume two, devices and nano-engineering, CRC Press, Boca RatonGoogle Scholar
- Bergman L, McHale JL (2011) Handbook of luminescent semiconductor materials, CRC Press, Boca RatonGoogle Scholar
- Joulaud C, Mugnier Y, Djanta G, Dubled M, Marty J-C, Galez C, Wolf J-P, Bonacina L, Le Dantec R (2013) Characterization of the nonlinear optical properties of nanocrystals by Hyper Rayleigh Scattering. J Nanobiotechnology 11:S8. doi:10.1186/1477-3155-11-S1-S8 View ArticleGoogle Scholar
- Andelman T, Gong Y, Polking M, Yin M, Kuskovsky I, Neumark G, O’Brien S (2005) Morphological control and photoluminescence of zinc oxide nanocrystals. J Phys Chem B 109:14314–14318. doi:10.1021/jp050540o View ArticleGoogle Scholar
- Pourrahimi AM, Liua D, Pallon LKH, Andersson RL, Martínez Abad A, Lagarón J-M, Hedenqvist MS, Ström V, Gedde UW, Olsson RT (2014) Water-based synthesis and cleaning methods for high purity ZnO nanoparticles—comparing acetate, chloride, sulphate and nitrate zinc salt precursors. RSC Adv 4:35568–35577. doi:10.1039/C4RA06651K View ArticleGoogle Scholar
- Gayvoronsky VYa, Popov AS, Brodyn MS, Uklein AV, Multian VV, Shul’zhenko OO (2015) The effect of sintering temperature on linear and nonlinear optical properties of YAG nanoceramics. In: Nanocomposites, nanophotonics, nanobiotechnology, and applications, vol 156. Springer, Cham, pp 147–164. doi:10.1007/978-3-319-06611-013
- Uklein AV, Popov AS, Multian VV, Brodyn MS, Kononets VV, Sidletskiy OT, Gayvoronsky VYa (2015) Photoinduced refractive index variation within picosecond laser pulses excitation as the indicator of oxyorthosilicates single crystals composition modification. Nanoscale Res Lett 10:102. doi:10.1186/s11671-015-0799-1
- Uklein AV, Diyuk VE, Grishchenko LM, Kozhanov VO, Boldyrieva OY, Lisnyak VV, Multian VV, Gayvoronsky VYa (2016) Characterization of oxidized carbon materials with photoinduced absorption response. Appl Phys B 122:287. doi:10.1007/s00340-016-6561-2
- Popov AI, Kotomin EA, Maier J (2010) Basic properties of the F-type centers in halides, oxides and perovskites. Nucl Instr Meth Phys Res B 268:3084–3089View ArticleGoogle Scholar
- Goh EG, Xu X, McCormick PG (2014) Effect of particle size on the UV absorbance of zinc oxide nanoparticles. Scr Mater 78:49–52. doi:10.1016/j.scriptamat.2014.01.033 View ArticleGoogle Scholar
- Satyanarayana Talam S, Karumuri SO, Gunnam N (2012) Synthesis, characterization, and spectroscopic properties of ZnO nanoparticles. ISRN Nanotechnology 2012:372505. doi:10.5402/2012/372505 Google Scholar
- Ye JD, Gu SL, Qin F, Zhu SM, Liu SM et al (2005) Correlation between green luminescence and morphology evolution of ZnO films. Appl Phys A 81:759–762. doi:10.1007/s00339-004-2996-0 View ArticleGoogle Scholar
- Zeng H, Duan G, Li Y, Yang S, Xu X, Cai W (2010) Blue luminescence of ZnO nanoparticles based on non-equilibrium processes: defect origins and emission controls. Adv Funct Mater 20:561–572. doi:10.1002/adfm.200901884 View ArticleGoogle Scholar
- Willander M, Nur O, Sadaf JR, Qadir MI, Zaman S, Zainelabdin A, Bano N, Hussain I (2010) Luminescence from zinc oxide nanostructures and polymers and their hybrid devices. Materials 3:2643–2667. doi:10.3390/ma3042643 View ArticleGoogle Scholar
- Bandopadhyay K, Mitra J (2015) Paper Zn interstitials and O vacancies responsible for n-type ZnO: what do the emission spectra reveal? RSC Adv 5:23540–23547. doi:10.1039/C5RA00355E View ArticleGoogle Scholar
- Xiong G, Pal U, Serrano JG, Ucer KB, Williams RT (2006) A photoluminescence and FTIR study of ZnO nanoparticles: the impurity and defect perspective. Phys Stat Sol C 3:3577–3581. doi:10.1002/pssc.200672164 View ArticleGoogle Scholar
- Jortner J (1994) Cluster size effects. Z Phys D 24:247–275. doi:10.1007/BF01425749 View ArticleGoogle Scholar
- Viswanatha R, Sapra S, Satpati B, Satyam PV, Dev BN, Sarma DD (2004) Understanding the quantum size effects in ZnO nanocrystals. J Mater Chem 14:661–668. doi:10.1039/B310404D View ArticleGoogle Scholar
- Brus L (1986) Electronic wave functions in semiconductor clusters: experiment and theory. J Phys Chem 90:2555–2560. doi:10.1021/j100403a003 View ArticleGoogle Scholar
- Asok A, Ghosh S, More PA, Chopade BA, Gandhi MN, Kulkarni AR (2015) Surface defect rich ZnO quantum dots as antioxidants inhibiting α-amylase and α-glucosidase: a potential anti-diabetic nanomedicine. J Mater Chem B 3:4597–4606. doi:10.1039/C5TB00407A View ArticleGoogle Scholar
- Camarda P, Messina F, Vaccaro L, Agnello S, Buscarino G, Schneider R, Popescu R, Gerthsen D, Lorenzi R, Gelardi FM, Cannas M (2016) Luminescence mechanisms of defective ZnO nanoparticles. Phys Chem Chem Phys 18:16237–16244. doi:10.1039/c6cp01513a View ArticleGoogle Scholar
- Collantes Y, Perales-Perez O (2013) Crystal size on the structural and functional properties of waterstable monodisperse ZnO nanoparticles synthesized via a polyol-route. Mater Res Soc Symp Proc 1551:117–122. doi:10.1557/opl.2013.901 Google Scholar
- Duchateau G, Geoffroy G, Dyan A, Piombini H, Guizard S (2011) Electron-hole dynamics in normal and deuterated KH2PO4 illuminated by intense femtosecond laser pulses. Phys Rev B 83:075114. doi:10.1103/PhysRevB.83.075114 View ArticleGoogle Scholar
- Gayvoronsky VYa, Kopylovsky MA, Brodyn MS, Pritula IM, Kolybaeva MI, Puzikov VM (2013) Impact of incorporated anatase nanoparticles on the second harmonic generation in KDP single crystals. Las Phys Lett 10:035401. doi:10.1088/1612-2011/10/3/035401
- Staedler D, Magouroux T, Hadji R, Joulaud C, Extermann J, Schwung S, Dantec RL et al (2012) Harmonic nanocrystals for biolabeling: a survey of optical properties and biocompatibility. ACS Nano 6:2542–2549. doi:10.1021/nn204990n View ArticleGoogle Scholar